Pipeline Hydro Test Pressure Determination
If test pressure reaching 100% (design factor of 0.80) of the SMYS is considered, then one must also consider some important pre conditions attached to the procurement of the steel and pipe. Especially important to consider is the level of flaw size that was accepted in the plate/coil used to manufacture the pipe. The test pressure of such magnitude would require that the acceptable defect size be re-assessed. This is because all else being equal, a higher design factor, resulting in a thinner wall, will lead to a reduction in the critical dimensions of both surface and through-wall defects.
Where such conditions are likely it may be prudent to reconsider the level of accepted flaws in the material. The current recommendations in API 5L 44th edition for acceptance level B2 as per ISO 12094 (for SAW pipes) may not be acceptable because it has limited coverage of body and edges and the acceptance criteria is far too liberal, in terms of acceptable size and area of flaws. More stringent criteria must be specified more in line with EN 10160 where level S2 for body and level E2 for edges may be more appropriate to meet the demands of the higher test pressures.
Sub-critical surface flaw sizes at design factors of 0.80 and 0.72 are susceptible to growth at low stress and are time dependent. These flaws are also dependent on the acceptable limits of impact absorbing energy of the material and weld (not part of the discussion in this article).
This increase in depth-to-thickness (d/t) ratio in effect reduces the ligament of the adjoining defects that reduce the required stress to propagate the discontinuity. Critical through-wall flaw lengths are also factors to be assessed. While there is a modest reduction in critical flaw length, it still indicates very acceptable flaw tolerance for any practical depth and the reduction will have negligible influence in the context of integrity management. Note that flaws deeper than about 70% of wall thickness will fail as stable leaks in both cases. This statement implies that mere radiography of the pipe welds (both field and mill welds) may not suffice. Automatic ultrasonic testing (AUT) of the welds will be better suited to properly determine the size of the planer defects in the welds. Similarly the use of AUT for assessing the flaws in the pipe body will be more stringent than usual.
The phenomenon of pressure reversal occurs when a defect survives a higher hydrostatic test pressure but fails at a lower pressure in a subsequent repressurization. One of the several factors that work to bring on this phenomenon is the creep-like growth of sub-critical discontinuities over time and at lower pressure. The reduction in the wall thickness, caused by corrosion, external damages, is also responsible for a reduction in puncture resistance in the pipe. The reduction in the wall thickness, in effect reduces the discontinuity depth to the material thickness.
- Coatings, pipe joint
- Compressor components
- Contractor, pipeline
- Contractor, river crossing/ directional drilling
- Directional drilling rigs, large
- Fittings, valves: plastic
- Meters, flow
- Pigs, cleaning
- Pigs, intelligent
- Pigs, scraper/ sphere launchers/ traps
- Scada systems
- Ultrasonic inspection
- Vacuum excavators/ potholing
- Valves, ball
- Welding systems, automatic